#------------------------------------------------------------------------------
#$Date: 2016-03-25 15:55:50 +0200 (Fri, 25 Mar 2016) $
#$Revision: 179943 $
#$URL: svn://www.crystallography.net/cod/cif/7/02/38/7023829.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7023829
loop_
_publ_author_name
'Shevchenko, Denys'
'Huang, Ping'
'Bon, Volodymyr V.'
'Anderlund, Magnus F.'
'Kokozay, Vladimir N.'
'Styring, Stenbjörn'
'Thapper, Anders'
_publ_section_title
;
 Synthesis, crystal structure, mass spectrometry, electrochemistry and
 magnetism of a Mn(III)-substituted trilacunary Keggin tungstosilicate.
;
_journal_issue                   14
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              5130
_journal_page_last               5139
_journal_paper_doi               10.1039/c3dt12500a
_journal_volume                  42
_journal_year                    2013
_chemical_formula_sum            'K4 Mn3 O51 Si W9'
_chemical_formula_weight         2819.96
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           11
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2yb'
_symmetry_space_group_name_H-M   'P 1 21/m 1'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 115.7400(10)
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   12.4191(2)
_cell_length_b                   15.6401(3)
_cell_length_c                   12.5526(2)
_cell_measurement_reflns_used    7918
_cell_measurement_temperature    173(2)
_cell_measurement_theta_max      26.50
_cell_measurement_theta_min      2.22
_cell_volume                     2196.24(7)
_computing_cell_refinement       'Bruker SAINT'
_computing_data_collection       'Bruker APEX2'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      173(2)
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0656
_diffrn_reflns_av_sigmaI/netI    0.0380
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_k_max       19
_diffrn_reflns_limit_k_min       -19
_diffrn_reflns_limit_l_max       15
_diffrn_reflns_limit_l_min       -15
_diffrn_reflns_number            33114
_diffrn_reflns_theta_full        26.56
_diffrn_reflns_theta_max         26.56
_diffrn_reflns_theta_min         1.82
_exptl_absorpt_coefficient_mu    24.827
_exptl_absorpt_correction_T_max  0.1991
_exptl_absorpt_correction_T_min  0.0578
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   'SADABS (Bruker, 2003)'
_exptl_crystal_colour            purple
_exptl_crystal_density_diffrn    4.264
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             2478
_exptl_crystal_size_max          0.27
_exptl_crystal_size_mid          0.15
_exptl_crystal_size_min          0.10
_refine_diff_density_max         2.616
_refine_diff_density_min         -2.128
_refine_diff_density_rms         0.333
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.093
_refine_ls_matrix_type           full
_refine_ls_number_parameters     331
_refine_ls_number_reflns         4753
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.093
_refine_ls_R_factor_all          0.0440
_refine_ls_R_factor_gt           0.0326
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0341P)²+31.8660P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0769
_refine_ls_wR_factor_ref         0.0832
_reflns_number_gt                4024
_reflns_number_total             4753
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c3dt12500a.cif
_cod_data_source_block           1071n
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Monoclinic' changed to 'monoclinic'
according to /home/saulius/struct/CIF-dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 1891 2012-01-12 08:04:46Z andrius 

The following automatic conversions were performed:

'_exptl_crystal_density_meas' value 'not measured' was changed to '?'
- the value is perceived as not measured.

Automatic conversion script
Id: cif_fix_values 3008 2015-01-20 13:52:24Z robertas 
;
_cod_original_sg_symbol_H-M      P2(1)/m
_cod_database_code               7023829
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y+1/2, -z'
'-x, -y, -z'
'x, -y-1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
W1 W 0.98835(5) 0.2500 0.97867(5) 0.01202(13) Uani 1 2 d S
W2 W 0.73859(4) 0.02604(2) 0.69411(4) 0.01320(10) Uani 1 1 d .
W3 W 0.70650(4) 0.13155(2) 0.91030(4) 0.01194(10) Uani 1 1 d .
W4 W 1.02337(4) 0.14267(2) 0.76061(4) 0.01320(10) Uani 1 1 d .
W5 W 0.77791(4) 0.14416(2) 0.45516(4) 0.01413(11) Uani 1 1 d .
Mn1 Mn 0.50146(12) 0.13693(8) 0.63963(12) 0.0067(3) Uani 1 1 d .
Mn2 Mn 0.54037(19) 0.2500 0.41060(19) 0.0134(4) Uani 1 2 d S
K1 K 0.2322(3) 0.2500 0.3737(3) 0.0266(8) Uani 1 2 d S
K2 K 1.0000 0.0000 1.0000 0.093(3) Uani 1 2 d S
K3 K 0.3685(3) 0.0138(2) 0.8253(3) 0.0415(8) Uani 1 1 d .
Si1 Si 0.7560(3) 0.2500 0.6940(3) 0.0066(7) Uani 1 2 d S
O1 O 0.8751(6) 0.1662(4) 0.9646(6) 0.0152(15) Uani 1 1 d .
O2 O 0.9012(8) 0.2500 0.7729(8) 0.0086(18) Uani 1 2 d S
O3 O 1.0713(6) 0.1644(4) 0.9277(6) 0.0161(15) Uani 1 1 d .
O4 O 1.0794(9) 0.2500 1.1263(8) 0.015(2) Uani 1 2 d S
O5 O 0.9066(6) 0.0673(4) 0.7633(6) 0.0175(15) Uani 1 1 d .
O6 O 0.9347(6) 0.1493(4) 0.5957(6) 0.0158(15) Uani 1 1 d .
O7 O 1.1003(9) 0.2500 0.7570(9) 0.019(2) Uani 1 2 d S
O8 O 1.1365(6) 0.0742(4) 0.7742(6) 0.0185(16) Uani 1 1 d .
O9 O 0.8240(8) 0.2500 0.4064(9) 0.017(2) Uani 1 2 d S
O10 O 0.8108(7) 0.0754(5) 0.3670(6) 0.0209(16) Uani 1 1 d .
O11 O 0.7296(9) 0.2500 0.5559(8) 0.014(2) Uani 1 2 d S
O12 O 0.7371(6) 0.0654(4) 0.5484(6) 0.0182(15) Uani 1 1 d .
O13 O 0.6177(6) 0.1646(5) 0.3598(6) 0.0188(15) Uani 1 1 d .
O14 O 0.7012(6) 0.1655(4) 0.7260(6) 0.0113(14) Uani 1 1 d .
O15 O 0.5730(6) 0.0280(4) 0.6336(6) 0.0172(15) Uani 1 1 d .
O16 O 0.7647(6) -0.0805(4) 0.6871(7) 0.0209(16) Uani 1 1 d .
O17 O 0.7555(6) 0.0283(4) 0.8536(6) 0.0171(15) Uani 1 1 d .
O18 O 0.5505(6) 0.1141(4) 0.8063(6) 0.0153(15) Uani 1 1 d .
O19 O 0.6831(8) 0.2500 0.9260(9) 0.014(2) Uani 1 2 d S
O20 O 0.7131(6) 0.0907(4) 1.0393(6) 0.0181(15) Uani 1 1 d .
O21 O 0.4490(10) 0.2500 0.6522(9) 0.021(2) Uani 1 2 d S
O22 O 0.4805(6) 0.1611(5) 0.4809(6) 0.0184(15) Uani 1 1 d .
O23 O 0.3764(9) 0.2500 0.2533(9) 0.023(2) Uani 1 2 d S
O24 O 0.3306(7) 0.0803(5) 0.5969(6) 0.0219(16) Uani 1 1 d .
O25 O 0.1116(10) 0.1502(9) 0.4880(12) 0.075(4) Uani 1 1 d .
O26 O 0.4658(11) 0.1132(10) 1.0151(13) 0.086(5) Uani 1 1 d .
O27 O 0.3457(13) 0.2500 0.8026(15) 0.074(6) Uani 1 2 d S
O28 O 0.7072(7) 0.8716(5) 0.9117(7) 0.0213(16) Uani 1 1 d .
O29 O 0.9722(8) 0.0932(5) 0.2428(12) 0.058(3) Uani 1 1 d .
O30 O 0.8555(9) 0.2500 0.2017(8) 0.012(2) Uani 1 2 d S
O31 O 0.6131(11) 0.2500 0.1325(10) 0.034(3) Uani 1 2 d S
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mn Mn 0.3368 0.7283 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O4 W1 O1 102.7(3) . .
O4 W1 O1 102.7(3) . 4_565
O1 W1 O1 88.8(4) . 4_565
O4 W1 O3 99.3(3) . 4_565
O1 W1 O3 158.0(3) . 4_565
O1 W1 O3 88.3(3) 4_565 4_565
O4 W1 O3 99.3(3) . .
O1 W1 O3 88.3(3) . .
O1 W1 O3 158.0(3) 4_565 .
O3 W1 O3 86.2(4) 4_565 .
O4 W1 O2 168.0(4) . .
O1 W1 O2 85.8(3) . .
O1 W1 O2 85.8(3) 4_565 .
O3 W1 O2 72.2(3) 4_565 .
O3 W1 O2 72.2(3) . .
O16 W2 O15 101.3(3) . .
O16 W2 O17 97.7(3) . .
O15 W2 O17 91.5(3) . .
O16 W2 O12 100.8(3) . .
O15 W2 O12 93.1(3) . .
O17 W2 O12 159.6(3) . .
O16 W2 O5 98.8(3) . .
O15 W2 O5 159.9(3) . .
O17 W2 O5 85.4(3) . .
O12 W2 O5 83.5(3) . .
O16 W2 O14 172.5(3) . .
O15 W2 O14 77.6(3) . .
O17 W2 O14 74.9(3) . .
O12 W2 O14 86.7(3) . .
O5 W2 O14 82.5(3) . .
O16 W2 Mn1 133.7(2) . .
O15 W2 Mn1 32.6(2) . .
O17 W2 Mn1 83.5(2) . .
O12 W2 Mn1 89.7(2) . .
O5 W2 Mn1 127.4(2) . .
O14 W2 Mn1 44.97(16) . .
O20 W3 O18 102.7(3) . .
O20 W3 O19 102.3(4) . .
O18 W3 O19 93.3(4) . .
O20 W3 O17 98.1(3) . .
O18 W3 O17 91.0(3) . .
O19 W3 O17 157.7(4) . .
O20 W3 O1 99.7(3) . .
O18 W3 O1 157.5(3) . .
O19 W3 O1 83.3(3) . .
O17 W3 O1 84.4(3) . .
O20 W3 O14 171.1(3) . .
O18 W3 O14 76.3(3) . .
O19 W3 O14 86.7(3) . .
O17 W3 O14 73.1(3) . .
O1 W3 O14 81.3(3) . .
O8 W4 O6 102.0(3) . .
O8 W4 O5 102.2(3) . .
O6 W4 O5 88.1(3) . .
O8 W4 O7 98.8(4) . .
O6 W4 O7 89.2(4) . .
O5 W4 O7 159.0(3) . .
O8 W4 O3 98.5(3) . .
O6 W4 O3 159.5(3) . .
O5 W4 O3 88.2(3) . .
O7 W4 O3 87.1(4) . .
O8 W4 O2 168.4(3) . .
O6 W4 O2 86.9(3) . .
O5 W4 O2 85.4(3) . .
O7 W4 O2 73.6(3) . .
O3 W4 O2 72.8(3) . .
O10 W5 O13 100.4(3) . .
O10 W5 O12 101.0(3) . .
O13 W5 O12 90.6(3) . .
O10 W5 O9 98.4(4) . .
O13 W5 O9 91.7(4) . .
O12 W5 O9 159.6(3) . .
O10 W5 O6 100.5(3) . .
O13 W5 O6 159.0(3) . .
O12 W5 O6 84.3(3) . .
O9 W5 O6 86.3(3) . .
O10 W5 O11 172.7(3) . .
O13 W5 O11 76.7(3) . .
O12 W5 O11 85.8(3) . .
O9 W5 O11 75.1(3) . .
O6 W5 O11 82.6(3) . .
O10 W5 Mn2 132.0(2) . .
O13 W5 Mn2 31.9(2) . .
O12 W5 Mn2 88.3(2) . .
O9 W5 Mn2 83.1(3) . .
O6 W5 Mn2 127.4(2) . .
O11 W5 Mn2 44.8(2) . .
O21 Mn1 O22 90.4(4) . .
O21 Mn1 O15 173.4(4) . .
O22 Mn1 O15 89.5(3) . .
O21 Mn1 O18 92.3(4) . .
O22 Mn1 O18 170.6(3) . .
O15 Mn1 O18 86.9(3) . .
O21 Mn1 O24 93.8(4) . .
O22 Mn1 O24 98.5(3) . .
O15 Mn1 O24 92.7(3) . .
O18 Mn1 O24 90.4(3) . .
O21 Mn1 O14 96.8(4) . .
O22 Mn1 O14 94.8(3) . .
O15 Mn1 O14 76.6(3) . .
O18 Mn1 O14 75.9(3) . .
O24 Mn1 O14 162.9(3) . .
O21 Mn1 W2 142.3(3) . .
O22 Mn1 W2 91.5(2) . .
O15 Mn1 W2 31.1(2) . .
O18 Mn1 W2 80.9(2) . .
O24 Mn1 W2 123.0(2) . .
O14 Mn1 W2 45.53(16) . .
O13 Mn2 O13 88.8(5) 4_565 .
O13 Mn2 O22 172.7(3) 4_565 .
O13 Mn2 O22 89.9(3) . .
O13 Mn2 O22 89.9(3) 4_565 4_565
O13 Mn2 O22 172.7(3) . 4_565
O22 Mn2 O22 90.5(4) . 4_565
O13 Mn2 O23 96.2(3) 4_565 .
O13 Mn2 O23 96.2(3) . .
O22 Mn2 O23 91.2(3) . .
O22 Mn2 O23 91.2(3) 4_565 .
O13 Mn2 O11 76.8(3) 4_565 .
O13 Mn2 O11 76.8(3) . .
O22 Mn2 O11 95.8(3) . .
O22 Mn2 O11 95.8(3) 4_565 .
O23 Mn2 O11 170.0(4) . .
O13 Mn2 W5 30.8(2) 4_565 4_565
O13 Mn2 W5 82.0(2) . 4_565
O22 Mn2 W5 141.9(2) . 4_565
O22 Mn2 W5 93.2(2) 4_565 4_565
O23 Mn2 W5 126.6(3) . 4_565
O11 Mn2 W5 46.07(17) . 4_565
O13 Mn2 W5 82.0(2) 4_565 .
O13 Mn2 W5 30.8(2) . .
O22 Mn2 W5 93.2(2) . .
O22 Mn2 W5 141.9(2) 4_565 .
O23 Mn2 W5 126.6(2) . .
O11 Mn2 W5 46.07(17) . .
W5 Mn2 W5 62.02(4) 4_565 .
O16 K1 O16 147.2(3) 3_656 2_656
O16 K1 O23 76.23(17) 3_656 .
O16 K1 O23 76.23(17) 2_656 .
O16 K1 O4 77.37(18) 3_656 1_454
O16 K1 O4 77.37(18) 2_656 1_454
O23 K1 O4 72.0(3) . 1_454
O16 K1 O25 135.8(3) 3_656 4_565
O16 K1 O25 72.3(3) 2_656 4_565
O23 K1 O25 147.8(3) . 4_565
O4 K1 O25 107.0(3) 1_454 4_565
O16 K1 O25 72.3(3) 3_656 .
O16 K1 O25 135.8(3) 2_656 .
O23 K1 O25 147.8(3) . .
O4 K1 O25 107.0(3) 1_454 .
O25 K1 O25 64.3(5) 4_565 .
O16 K1 O22 114.8(2) 3_656 4_565
O16 K1 O22 63.9(2) 2_656 4_565
O23 K1 O22 59.1(2) . 4_565
O4 K1 O22 122.5(2) 1_454 4_565
O25 K1 O22 99.9(3) 4_565 4_565
O25 K1 O22 130.4(3) . 4_565
O16 K1 O22 63.9(2) 3_656 .
O16 K1 O22 114.8(2) 2_656 .
O23 K1 O22 59.1(2) . .
O4 K1 O22 122.5(2) 1_454 .
O25 K1 O22 130.4(3) 4_565 .
O25 K1 O22 99.9(3) . .
O22 K1 O22 53.2(3) 4_565 .
O16 K1 O21 100.76(18) 3_656 .
O16 K1 O21 100.76(18) 2_656 .
O23 K1 O21 98.7(3) . .
O4 K1 O21 170.7(3) 1_454 .
O25 K1 O21 80.8(3) 4_565 .
O25 K1 O21 80.8(3) . .
O22 K1 O21 49.7(2) 4_565 .
O22 K1 O21 49.7(2) . .
O17 K2 O17 180.0(3) 3_757 .
O17 K2 O5 55.4(2) 3_757 3_757
O17 K2 O5 124.6(2) . 3_757
O17 K2 O5 124.6(2) 3_757 .
O17 K2 O5 55.4(2) . .
O5 K2 O5 180.000(1) 3_757 .
O17 K2 O1 54.42(19) 3_757 3_757
O17 K2 O1 125.58(19) . 3_757
O5 K2 O1 64.78(19) 3_757 3_757
O5 K2 O1 115.22(19) . 3_757
O17 K2 O1 125.58(19) 3_757 .
O17 K2 O1 54.42(19) . .
O5 K2 O1 115.22(19) 3_757 .
O5 K2 O1 64.78(19) . .
O1 K2 O1 179.999(1) 3_757 .
O17 K2 O3 92.52(19) 3_757 3_757
O17 K2 O3 87.47(19) . 3_757
O5 K2 O3 53.92(19) 3_757 3_757
O5 K2 O3 126.08(19) . 3_757
O1 K2 O3 53.37(18) 3_757 3_757
O1 K2 O3 126.63(18) . 3_757
O17 K2 O3 87.48(19) 3_757 .
O17 K2 O3 92.53(19) . .
O5 K2 O3 126.08(19) 3_757 .
O5 K2 O3 53.92(19) . .
O1 K2 O3 126.63(18) 3_757 .
O1 K2 O3 53.37(18) . .
O3 K2 O3 179.999(1) 3_757 .
O26 K3 O8 91.7(3) . 1_455
O26 K3 O10 159.0(3) . 3_656
O8 K3 O10 68.0(2) 1_455 3_656
O26 K3 O20 86.6(4) . 3_657
O8 K3 O20 74.6(2) 1_455 3_657
O10 K3 O20 82.8(2) 3_656 3_657
O26 K3 O18 71.6(3) . .
O8 K3 O18 124.4(2) 1_455 .
O10 K3 O18 123.9(2) 3_656 .
O20 K3 O18 150.4(2) 3_657 .
O26 K3 O24 119.6(4) . .
O8 K3 O24 86.8(2) 1_455 .
O10 K3 O24 66.7(2) 3_656 .
O20 K3 O24 148.6(2) 3_657 .
O18 K3 O24 60.8(2) . .
O26 K3 O26 82.7(4) . 3_657
O8 K3 O26 136.4(3) 1_455 3_657
O10 K3 O26 107.9(3) 3_656 3_657
O20 K3 O26 61.9(3) 3_657 3_657
O18 K3 O26 94.8(3) . 3_657
O24 K3 O26 133.2(3) . 3_657
O14 Si1 O14 109.8(5) . 4_565
O14 Si1 O11 110.8(3) . .
O14 Si1 O11 110.8(3) 4_565 .
O14 Si1 O2 108.8(3) . .
O14 Si1 O2 108.8(3) 4_565 .
O11 Si1 O2 107.8(5) . .
W1 O1 W3 149.8(4) . .
W1 O1 K2 106.1(3) . .
W3 O1 K2 102.6(3) . .
Si1 O2 W4 122.8(3) . 4_565
Si1 O2 W4 122.8(3) . .
W4 O2 W4 93.1(3) 4_565 .
Si1 O2 W1 122.0(5) . .
W4 O2 W1 94.1(3) 4_565 .
W4 O2 W1 94.1(3) . .
W4 O3 W1 120.9(4) . .
W4 O3 K2 100.6(3) . .
W1 O3 K2 102.8(3) . .
W1 O4 K1 179.9(6) . 1_656
W4 O5 W2 150.1(4) . .
W4 O5 K2 106.2(3) . .
W2 O5 K2 102.0(3) . .
W4 O6 W5 149.1(4) . .
W4 O7 W4 119.7(5) 4_565 .
W4 O8 K3 160.2(4) . 1_655
W5 O9 W5 117.6(5) 4_565 .
W5 O10 K3 122.5(4) . 3_656
Si1 O11 Mn2 121.3(5) . .
Si1 O11 W5 127.2(3) . 4_565
Mn2 O11 W5 89.1(3) . 4_565
Si1 O11 W5 127.2(3) . .
Mn2 O11 W5 89.1(3) . .
W5 O11 W5 91.3(3) 4_565 .
W5 O12 W2 153.2(4) . .
W5 O13 Mn2 117.4(4) . .
Si1 O14 Mn1 122.1(4) . .
Si1 O14 W2 126.4(4) . .
Mn1 O14 W2 89.5(2) . .
Si1 O14 W3 126.6(4) . .
Mn1 O14 W3 89.0(2) . .
W2 O14 W3 92.0(2) . .
W2 O15 Mn1 116.3(3) . .
W2 O16 K1 167.5(4) . 3_656
W2 O17 W3 118.8(3) . .
W2 O17 K2 106.0(3) . .
W3 O17 K2 108.0(3) . .
W3 O18 Mn1 118.8(4) . .
W3 O18 K3 131.1(3) . .
Mn1 O18 K3 107.6(3) . .
W3 O19 W3 154.7(6) 4_565 .
W3 O20 K3 153.9(4) . 3_657
Mn1 O21 Mn1 134.9(6) 4_565 .
Mn1 O21 K1 93.5(3) 4_565 .
Mn1 O21 K1 93.5(3) . .
Mn1 O22 Mn2 134.1(4) . .
Mn1 O22 K1 101.4(3) . .
Mn2 O22 K1 89.2(3) . .
Mn2 O23 K1 94.5(4) . .
Mn1 O24 K3 100.6(3) . .
K3 O26 K3 97.3(4) . 3_657
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
W1 O4 1.700(9) .
W1 O1 1.874(7) .
W1 O1 1.874(7) 4_565
W1 O3 1.958(7) 4_565
W1 O3 1.958(7) .
W1 O2 2.327(9) .
W2 O16 1.707(7) .
W2 O15 1.858(7) .
W2 O17 1.921(7) .
W2 O12 1.922(7) .
W2 O5 1.988(7) .
W2 O14 2.301(6) .
W2 Mn1 3.2247(14) .
W3 O20 1.709(7) .
W3 O18 1.826(7) .
W3 O19 1.899(2) .
W3 O17 1.964(7) .
W3 O1 1.976(7) .
W3 O14 2.346(7) .
W4 O8 1.715(7) .
W4 O6 1.878(7) .
W4 O5 1.880(7) .
W4 O7 1.941(5) .
W4 O3 1.945(7) .
W4 O2 2.312(6) .
W5 O10 1.715(7) .
W5 O13 1.850(7) .
W5 O12 1.913(7) .
W5 O9 1.936(5) .
W5 O6 1.982(7) .
W5 O11 2.314(7) .
W5 Mn2 3.2128(19) .
Mn1 O21 1.915(4) .
Mn1 O22 1.932(7) .
Mn1 O15 1.938(7) .
Mn1 O18 1.942(7) .
Mn1 O24 2.142(7) .
Mn1 O14 2.279(6) .
Mn2 O13 1.910(7) 4_565
Mn2 O13 1.910(7) .
Mn2 O22 1.958(7) .
Mn2 O22 1.958(7) 4_565
Mn2 O23 2.134(10) .
Mn2 O11 2.264(10) .
Mn2 W5 3.2128(19) 4_565
K1 O16 2.764(7) 3_656
K1 O16 2.764(7) 2_656
K1 O23 2.800(12) .
K1 O4 2.852(10) 1_454
K1 O25 2.933(12) 4_565
K1 O25 2.933(12) .
K1 O22 3.106(8) 4_565
K1 O22 3.106(8) .
K1 O21 3.360(11) .
K2 O17 2.819(7) 3_757
K2 O17 2.819(7) .
K2 O5 2.879(7) 3_757
K2 O5 2.879(7) .
K2 O1 2.960(7) 3_757
K2 O1 2.960(7) .
K2 O3 2.987(7) 3_757
K2 O3 2.987(7) .
K3 O26 2.657(13) .
K3 O8 2.829(8) 1_455
K3 O10 2.839(8) 3_656
K3 O20 2.843(8) 3_657
K3 O18 2.845(7) .
K3 O24 2.890(8) .
K3 O26 2.934(17) 3_657
Si1 O14 1.615(7) .
Si1 O14 1.615(7) 4_565
Si1 O11 1.619(10) .
Si1 O2 1.637(9) .
O2 W4 2.312(6) 4_565
O4 K1 2.852(10) 1_656
O7 W4 1.941(5) 4_565
O8 K3 2.829(8) 1_655
O9 W5 1.936(5) 4_565
O10 K3 2.839(8) 3_656
O11 W5 2.314(7) 4_565
O16 K1 2.764(7) 3_656
O19 W3 1.899(2) 4_565
O20 K3 2.843(8) 3_657
O21 Mn1 1.915(4) 4_565
O26 K3 2.934(17) 3_657
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
O16 W2 Mn1 O21 172.4(6) . .
O15 W2 Mn1 O21 -179.0(7) . .
O17 W2 Mn1 O21 77.9(5) . .
O12 W2 Mn1 O21 -82.8(5) . .
O5 W2 Mn1 O21 -1.2(6) . .
O14 W2 Mn1 O21 2.8(6) . .
O16 W2 Mn1 O22 -95.1(4) . .
O15 W2 Mn1 O22 -86.5(5) . .
O17 W2 Mn1 O22 170.4(3) . .
O12 W2 Mn1 O22 9.7(3) . .
O5 W2 Mn1 O22 91.2(3) . .
O14 W2 Mn1 O22 95.3(3) . .
O16 W2 Mn1 O15 -8.5(5) . .
O17 W2 Mn1 O15 -103.1(5) . .
O12 W2 Mn1 O15 96.2(5) . .
O5 W2 Mn1 O15 177.8(5) . .
O14 W2 Mn1 O15 -178.2(5) . .
O16 W2 Mn1 O18 90.5(4) . .
O15 W2 Mn1 O18 99.1(5) . .
O17 W2 Mn1 O18 -4.0(3) . .
O12 W2 Mn1 O18 -164.7(3) . .
O5 W2 Mn1 O18 -83.1(3) . .
O14 W2 Mn1 O18 -79.1(3) . .
O16 W2 Mn1 O24 6.0(4) . .
O15 W2 Mn1 O24 14.6(5) . .
O17 W2 Mn1 O24 -88.5(3) . .
O12 W2 Mn1 O24 110.8(3) . .
O5 W2 Mn1 O24 -167.6(3) . .
O14 W2 Mn1 O24 -163.6(3) . .
O16 W2 Mn1 O14 169.6(4) . .
O15 W2 Mn1 O14 178.2(5) . .
O17 W2 Mn1 O14 75.1(3) . .
O12 W2 Mn1 O14 -85.6(3) . .
O5 W2 Mn1 O14 -4.1(3) . .
O10 W5 Mn2 O13 -91.6(4) . 4_565
O13 W5 Mn2 O13 -101.2(6) . 4_565
O12 W5 Mn2 O13 165.0(3) . 4_565
O9 W5 Mn2 O13 3.5(4) . 4_565
O6 W5 Mn2 O13 83.5(3) . 4_565
O11 W5 Mn2 O13 79.3(3) . 4_565
O10 W5 Mn2 O13 9.6(5) . .
O12 W5 Mn2 O13 -93.9(5) . .
O9 W5 Mn2 O13 104.7(5) . .
O6 W5 Mn2 O13 -175.4(5) . .
O11 W5 Mn2 O13 -179.5(5) . .
O10 W5 Mn2 O22 94.0(4) . .
O13 W5 Mn2 O22 84.4(5) . .
O12 W5 Mn2 O22 -9.4(3) . .
O9 W5 Mn2 O22 -170.9(4) . .
O6 W5 Mn2 O22 -90.9(3) . .
O11 W5 Mn2 O22 -95.1(3) . .
O10 W5 Mn2 O22 -171.1(5) . 4_565
O13 W5 Mn2 O22 179.3(6) . 4_565
O12 W5 Mn2 O22 85.4(4) . 4_565
O9 W5 Mn2 O22 -76.0(5) . 4_565
O6 W5 Mn2 O22 3.9(4) . 4_565
O11 W5 Mn2 O22 -0.2(4) . 4_565
O10 W5 Mn2 O23 0.2(4) . .
O13 W5 Mn2 O23 -9.4(5) . .
O12 W5 Mn2 O23 -103.2(3) . .
O9 W5 Mn2 O23 95.3(4) . .
O6 W5 Mn2 O23 175.3(4) . .
O11 W5 Mn2 O23 171.1(4) . .
O10 W5 Mn2 O11 -170.9(4) . .
O13 W5 Mn2 O11 179.5(5) . .
O12 W5 Mn2 O11 85.7(3) . .
O9 W5 Mn2 O11 -75.8(4) . .
O6 W5 Mn2 O11 4.1(3) . .
O10 W5 Mn2 W5 -116.3(3) . 4_565
O13 W5 Mn2 W5 -125.9(4) . 4_565
O12 W5 Mn2 W5 140.3(2) . 4_565
O9 W5 Mn2 W5 -21.2(3) . 4_565
O6 W5 Mn2 W5 58.7(3) . 4_565
O11 W5 Mn2 W5 54.6(2) . 4_565
O4 W1 O1 W3 126.1(8) . .
O1 W1 O1 W3 23.4(10) 4_565 .
O3 W1 O1 W3 -59.1(13) 4_565 .
O3 W1 O1 W3 -134.7(8) . .
O2 W1 O1 W3 -62.5(8) . .
O4 W1 O1 K2 -72.5(3) . .
O1 W1 O1 K2 -175.2(3) 4_565 .
O3 W1 O1 K2 102.3(7) 4_565 .
O3 W1 O1 K2 26.6(3) . .
O2 W1 O1 K2 98.9(3) . .
O20 W3 O1 W1 -127.4(8) . .
O18 W3 O1 W1 56.4(12) . .
O19 W3 O1 W1 -26.0(8) . .
O17 W3 O1 W1 135.3(8) . .
O14 W3 O1 W1 61.6(8) . .
O20 W3 O1 K2 71.0(3) . .
O18 W3 O1 K2 -105.2(7) . .
O19 W3 O1 K2 172.3(4) . .
O17 W3 O1 K2 -26.3(3) . .
O14 W3 O1 K2 -100.1(2) . .
O17 K2 O1 W1 31.7(4) 3_757 .
O17 K2 O1 W1 -148.3(4) . .
O5 K2 O1 W1 96.0(3) 3_757 .
O5 K2 O1 W1 -84.0(3) . .
O1 K2 O1 W1 -4(17) 3_757 .
O3 K2 O1 W1 158.5(2) 3_757 .
O3 K2 O1 W1 -21.5(2) . .
O17 K2 O1 W3 -157.8(2) 3_757 .
O17 K2 O1 W3 22.2(2) . .
O5 K2 O1 W3 -93.5(3) 3_757 .
O5 K2 O1 W3 86.5(3) . .
O1 K2 O1 W3 166(17) 3_757 .
O3 K2 O1 W3 -30.9(4) 3_757 .
O3 K2 O1 W3 149.1(4) . .
O14 Si1 O2 W4 180.0(4) . 4_565
O14 Si1 O2 W4 -60.5(6) 4_565 4_565
O11 Si1 O2 W4 59.7(4) . 4_565
O14 Si1 O2 W4 60.5(6) . .
O14 Si1 O2 W4 -180.0(4) 4_565 .
O11 Si1 O2 W4 -59.7(4) . .
O14 Si1 O2 W1 -59.8(3) . .
O14 Si1 O2 W1 59.8(3) 4_565 .
O11 Si1 O2 W1 180.0 . .
O8 W4 O2 Si1 -175.9(13) . .
O6 W4 O2 Si1 44.2(5) . .
O5 W4 O2 Si1 -44.1(5) . .
O7 W4 O2 Si1 134.3(6) . .
O3 W4 O2 Si1 -133.6(5) . .
O8 W4 O2 W4 51.2(17) . 4_565
O6 W4 O2 W4 -88.7(3) . 4_565
O5 W4 O2 W4 -177.0(3) . 4_565
O7 W4 O2 W4 1.4(4) . 4_565
O3 W4 O2 W4 93.5(3) . 4_565
O8 W4 O2 W1 -43.1(16) . .
O6 W4 O2 W1 177.0(3) . .
O5 W4 O2 W1 88.6(3) . .
O7 W4 O2 W1 -93.0(4) . .
O3 W4 O2 W1 -0.8(2) . .
O4 W1 O2 Si1 180.000(4) . .
O1 W1 O2 Si1 44.5(2) . .
O1 W1 O2 Si1 -44.5(2) 4_565 .
O3 W1 O2 Si1 -134.1(2) 4_565 .
O3 W1 O2 Si1 134.1(2) . .
O4 W1 O2 W4 -46.71(17) . 4_565
O1 W1 O2 W4 177.8(3) . 4_565
O1 W1 O2 W4 88.8(3) 4_565 4_565
O3 W1 O2 W4 -0.8(2) 4_565 4_565
O3 W1 O2 W4 -92.6(3) . 4_565
O4 W1 O2 W4 46.71(17) . .
O1 W1 O2 W4 -88.8(3) . .
O1 W1 O2 W4 -177.8(3) 4_565 .
O3 W1 O2 W4 92.6(3) 4_565 .
O3 W1 O2 W4 0.8(2) . .
O8 W4 O3 W1 173.3(4) . .
O6 W4 O3 W1 -5.0(11) . .
O5 W4 O3 W1 -84.6(4) . .
O7 W4 O3 W1 74.9(4) . .
O2 W4 O3 W1 1.2(3) . .
O8 W4 O3 K2 -74.7(3) . .
O6 W4 O3 K2 107.0(8) . .
O5 W4 O3 K2 27.4(3) . .
O7 W4 O3 K2 -173.1(3) . .
O2 W4 O3 K2 113.2(3) . .
O4 W1 O3 W4 -172.5(4) . .
O1 W1 O3 W4 85.0(4) . .
O1 W1 O3 W4 2.4(10) 4_565 .
O3 W1 O3 W4 -73.7(4) 4_565 .
O2 W1 O3 W4 -1.2(3) . .
O4 W1 O3 K2 76.6(3) . .
O1 W1 O3 K2 -25.9(3) . .
O1 W1 O3 K2 -108.5(7) 4_565 .
O3 W1 O3 K2 175.4(3) 4_565 .
O2 W1 O3 K2 -112.1(3) . .
O17 K2 O3 W4 115.5(3) 3_757 .
O17 K2 O3 W4 -64.5(3) . .
O5 K2 O3 W4 158.2(2) 3_757 .
O5 K2 O3 W4 -21.8(2) . .
O1 K2 O3 W4 74.8(3) 3_757 .
O1 K2 O3 W4 -105.2(3) . .
O3 K2 O3 W4 40(4) 3_757 .
O17 K2 O3 W1 -119.2(3) 3_757 .
O17 K2 O3 W1 60.8(3) . .
O5 K2 O3 W1 -76.4(3) 3_757 .
O5 K2 O3 W1 103.6(3) . .
O1 K2 O3 W1 -159.8(2) 3_757 .
O1 K2 O3 W1 20.2(2) . .
O3 K2 O3 W1 165(4) 3_757 .
O1 W1 O4 K1 134(100) . 1_656
O1 W1 O4 K1 -134(100) 4_565 1_656
O3 W1 O4 K1 -44(100) 4_565 1_656
O3 W1 O4 K1 44(100) . 1_656
O2 W1 O4 K1 0(100) . 1_656
O8 W4 O5 W2 -130.6(8) . .
O6 W4 O5 W2 -28.7(8) . .
O7 W4 O5 W2 54.0(15) . .
O3 W4 O5 W2 131.1(8) . .
O2 W4 O5 W2 58.3(8) . .
O8 W4 O5 K2 69.1(3) . .
O6 W4 O5 K2 170.9(3) . .
O7 W4 O5 K2 -106.4(10) . .
O3 W4 O5 K2 -29.3(3) . .
O2 W4 O5 K2 -102.1(3) . .
O16 W2 O5 W4 129.6(8) . .
O15 W2 O5 W4 -51.5(14) . .
O17 W2 O5 W4 -133.3(8) . .
O12 W2 O5 W4 29.6(8) . .
O14 W2 O5 W4 -57.9(8) . .
Mn1 W2 O5 W4 -55.0(9) . .
O16 W2 O5 K2 -69.7(3) . .
O15 W2 O5 K2 109.2(8) . .
O17 W2 O5 K2 27.5(3) . .
O12 W2 O5 K2 -169.6(3) . .
O14 W2 O5 K2 102.8(3) . .
Mn1 W2 O5 K2 105.7(2) . .
O17 K2 O5 W4 -32.2(4) 3_757 .
O17 K2 O5 W4 147.8(4) . .
O5 K2 O5 W4 68(36) 3_757 .
O1 K2 O5 W4 -95.0(3) 3_757 .
O1 K2 O5 W4 85.0(3) . .
O3 K2 O5 W4 -156.8(2) 3_757 .
O3 K2 O5 W4 23.2(2) . .
O17 K2 O5 W2 157.6(2) 3_757 .
O17 K2 O5 W2 -22.4(2) . .
O5 K2 O5 W2 -103(36) 3_757 .
O1 K2 O5 W2 94.8(3) 3_757 .
O1 K2 O5 W2 -85.2(3) . .
O3 K2 O5 W2 33.0(4) 3_757 .
O3 K2 O5 W2 -147.0(4) . .
O8 W4 O6 W5 131.2(7) . .
O5 W4 O6 W5 29.1(7) . .
O7 W4 O6 W5 -130.0(8) . .
O3 W4 O6 W5 -50.5(13) . .
O2 W4 O6 W5 -56.4(7) . .
O10 W5 O6 W4 -130.7(7) . .
O13 W5 O6 W4 46.2(13) . .
O12 W5 O6 W4 -30.5(7) . .
O9 W5 O6 W4 131.4(8) . .
O11 W5 O6 W4 56.0(7) . .
Mn2 W5 O6 W4 53.0(8) . .
O8 W4 O7 W4 -172.9(5) . 4_565
O6 W4 O7 W4 85.1(6) . 4_565
O5 W4 O7 W4 2.6(15) . 4_565
O3 W4 O7 W4 -74.7(6) . 4_565
O2 W4 O7 W4 -1.9(5) . 4_565
O6 W4 O8 K3 112.2(11) . 1_655
O5 W4 O8 K3 -157.1(11) . 1_655
O7 W4 O8 K3 21.2(12) . 1_655
O3 W4 O8 K3 -67.2(12) . 1_655
O2 W4 O8 K3 -27(2) . 1_655
O10 W5 O9 W5 168.3(5) . 4_565
O13 W5 O9 W5 67.5(5) . 4_565
O12 W5 O9 W5 -29.0(13) . 4_565
O6 W5 O9 W5 -91.6(5) . 4_565
O11 W5 O9 W5 -8.2(5) . 4_565
Mn2 W5 O9 W5 36.8(5) . 4_565
O13 W5 O10 K3 -17.9(5) . 3_656
O12 W5 O10 K3 74.8(4) . 3_656
O9 W5 O10 K3 -111.3(4) . 3_656
O6 W5 O10 K3 160.9(4) . 3_656
O11 W5 O10 K3 -84(3) . 3_656
Mn2 W5 O10 K3 -23.1(6) . 3_656
O14 Si1 O11 Mn2 61.1(3) . .
O14 Si1 O11 Mn2 -61.1(3) 4_565 .
O2 Si1 O11 Mn2 180.000(1) . .
O14 Si1 O11 W5 177.1(5) . 4_565
O14 Si1 O11 W5 54.9(7) 4_565 4_565
O2 Si1 O11 W5 -64.0(5) . 4_565
O14 Si1 O11 W5 -54.9(7) . .
O14 Si1 O11 W5 -177.1(5) 4_565 .
O2 Si1 O11 W5 64.0(5) . .
O13 Mn2 O11 Si1 134.1(2) 4_565 .
O13 Mn2 O11 Si1 -134.1(2) . .
O22 Mn2 O11 Si1 -45.6(2) . .
O22 Mn2 O11 Si1 45.5(2) 4_565 .
O23 Mn2 O11 Si1 180.000(7) . .
W5 Mn2 O11 Si1 134.33(17) 4_565 .
W5 Mn2 O11 Si1 -134.32(17) . .
O13 Mn2 O11 W5 -0.3(3) 4_565 4_565
O13 Mn2 O11 W5 91.6(3) . 4_565
O22 Mn2 O11 W5 -179.9(3) . 4_565
O22 Mn2 O11 W5 -88.8(3) 4_565 4_565
O23 Mn2 O11 W5 45.67(17) . 4_565
W5 Mn2 O11 W5 91.3(3) . 4_565
O13 Mn2 O11 W5 -91.6(3) 4_565 .
O13 Mn2 O11 W5 0.3(3) . .
O22 Mn2 O11 W5 88.8(3) . .
O22 Mn2 O11 W5 179.9(3) 4_565 .
O23 Mn2 O11 W5 -45.68(17) . .
W5 Mn2 O11 W5 -91.3(3) 4_565 .
O10 W5 O11 Si1 -163(2) . .
O13 W5 O11 Si1 129.5(6) . .
O12 W5 O11 Si1 37.9(6) . .
O9 W5 O11 Si1 -135.0(7) . .
O6 W5 O11 Si1 -46.9(6) . .
Mn2 W5 O11 Si1 129.8(7) . .
O10 W5 O11 Mn2 67(3) . .
O13 W5 O11 Mn2 -0.3(3) . .
O12 W5 O11 Mn2 -91.9(3) . .
O9 W5 O11 Mn2 95.2(3) . .
O6 W5 O11 Mn2 -176.7(3) . .
O10 W5 O11 W5 -22(3) . 4_565
O13 W5 O11 W5 -89.4(3) . 4_565
O12 W5 O11 W5 179.0(3) . 4_565
O9 W5 O11 W5 6.1(3) . 4_565
O6 W5 O11 W5 94.2(3) . 4_565
Mn2 W5 O11 W5 -89.1(3) . 4_565
O10 W5 O12 W2 139.4(9) . .
O13 W5 O12 W2 -119.9(9) . .
O9 W5 O12 W2 -23.2(16) . .
O6 W5 O12 W2 39.7(9) . .
O11 W5 O12 W2 -43.3(9) . .
Mn2 W5 O12 W2 -88.1(9) . .
O16 W2 O12 W5 -136.9(9) . .
O15 W2 O12 W5 120.9(9) . .
O17 W2 O12 W5 18.1(16) . .
O5 W2 O12 W5 -39.2(9) . .
O14 W2 O12 W5 43.6(9) . .
Mn1 W2 O12 W5 88.5(9) . .
O10 W5 O13 Mn2 -172.8(4) . .
O12 W5 O13 Mn2 85.9(4) . .
O9 W5 O13 Mn2 -73.9(5) . .
O6 W5 O13 Mn2 10.3(11) . .
O11 W5 O13 Mn2 0.4(4) . .
O13 Mn2 O13 W5 76.4(5) 4_565 .
O22 Mn2 O13 W5 -96.4(4) . .
O22 Mn2 O13 W5 -3(3) 4_565 .
O23 Mn2 O13 W5 172.5(4) . .
O11 Mn2 O13 W5 -0.4(4) . .
W5 Mn2 O13 W5 46.3(4) 4_565 .
O14 Si1 O14 Mn1 60.7(6) 4_565 .
O11 Si1 O14 Mn1 -62.1(5) . .
O2 Si1 O14 Mn1 179.6(4) . .
O14 Si1 O14 W2 177.42(10) 4_565 .
O11 Si1 O14 W2 54.6(6) . .
O2 Si1 O14 W2 -63.7(5) . .
O14 Si1 O14 W3 -55.5(6) 4_565 .
O11 Si1 O14 W3 -178.3(4) . .
O2 Si1 O14 W3 63.4(5) . .
O21 Mn1 O14 Si1 -44.2(5) . .
O22 Mn1 O14 Si1 46.7(5) . .
O15 Mn1 O14 Si1 135.0(5) . .
O18 Mn1 O14 Si1 -134.9(5) . .
O24 Mn1 O14 Si1 -172.3(7) . .
W2 Mn1 O14 Si1 134.0(5) . .
O21 Mn1 O14 W2 -178.3(3) . .
O22 Mn1 O14 W2 -87.3(3) . .
O15 Mn1 O14 W2 1.0(3) . .
O18 Mn1 O14 W2 91.1(3) . .
O24 Mn1 O14 W2 53.6(9) . .
O21 Mn1 O14 W3 89.7(3) . .
O22 Mn1 O14 W3 -179.4(3) . .
O15 Mn1 O14 W3 -91.1(3) . .
O18 Mn1 O14 W3 -1.0(2) . .
O24 Mn1 O14 W3 -38.4(9) . .
W2 Mn1 O14 W3 -92.1(2) . .
O16 W2 O14 Si1 146(2) . .
O15 W2 O14 Si1 -131.8(5) . .
O17 W2 O14 Si1 133.2(5) . .
O12 W2 O14 Si1 -37.9(5) . .
O5 W2 O14 Si1 45.9(5) . .
Mn1 W2 O14 Si1 -130.8(5) . .
O16 W2 O14 Mn1 -83(2) . .
O15 W2 O14 Mn1 -1.0(3) . .
O17 W2 O14 Mn1 -96.0(3) . .
O12 W2 O14 Mn1 92.9(3) . .
O5 W2 O14 Mn1 176.7(3) . .
O16 W2 O14 W3 6(2) . .
O15 W2 O14 W3 88.0(3) . .
O17 W2 O14 W3 -7.0(3) . .
O12 W2 O14 W3 -178.1(3) . .
O5 W2 O14 W3 -94.2(3) . .
Mn1 W2 O14 W3 89.0(2) . .
O20 W3 O14 Si1 -143.8(17) . .
O18 W3 O14 Si1 131.5(5) . .
O19 W3 O14 Si1 37.3(5) . .
O17 W3 O14 Si1 -133.1(5) . .
O1 W3 O14 Si1 -46.4(5) . .
O20 W3 O14 Mn1 85.7(19) . .
O18 W3 O14 Mn1 1.0(3) . .
O19 W3 O14 Mn1 -93.2(3) . .
O17 W3 O14 Mn1 96.4(3) . .
O1 W3 O14 Mn1 -176.9(3) . .
O20 W3 O14 W2 -4(2) . .
O18 W3 O14 W2 -88.4(3) . .
O19 W3 O14 W2 177.3(3) . .
O17 W3 O14 W2 6.9(2) . .
O1 W3 O14 W2 93.6(3) . .
O16 W2 O15 Mn1 173.7(4) . .
O17 W2 O15 Mn1 75.5(4) . .
O12 W2 O15 Mn1 -84.6(4) . .
O5 W2 O15 Mn1 -5.2(11) . .
O14 W2 O15 Mn1 1.3(3) . .
O21 Mn1 O15 W2 5(3) . .
O22 Mn1 O15 W2 93.7(4) . .
O18 Mn1 O15 W2 -77.6(4) . .
O24 Mn1 O15 W2 -167.8(4) . .
O14 Mn1 O15 W2 -1.3(3) . .
O15 W2 O16 K1 47.6(19) . 3_656
O17 W2 O16 K1 140.7(18) . 3_656
O12 W2 O16 K1 -47.8(19) . 3_656
O5 W2 O16 K1 -132.8(18) . 3_656
O14 W2 O16 K1 128(2) . 3_656
Mn1 W2 O16 K1 52(2) . 3_656
O16 W2 O17 W3 -168.8(4) . .
O15 W2 O17 W3 -67.1(4) . .
O12 W2 O17 W3 36.0(11) . .
O5 W2 O17 W3 93.0(4) . .
O14 W2 O17 W3 9.5(3) . .
Mn1 W2 O17 W3 -35.5(3) . .
O16 W2 O17 K2 69.6(3) . .
O15 W2 O17 K2 171.2(3) . .
O12 W2 O17 K2 -85.7(9) . .
O5 W2 O17 K2 -28.6(3) . .
O14 W2 O17 K2 -112.1(3) . .
Mn1 W2 O17 K2 -157.1(2) . .
O20 W3 O17 W2 168.9(4) . .
O18 W3 O17 W2 65.9(4) . .
O19 W3 O17 W2 -35.3(11) . .
O1 W3 O17 W2 -92.1(4) . .
O14 W3 O17 W2 -9.4(3) . .
O20 W3 O17 K2 -70.5(3) . .
O18 W3 O17 K2 -173.5(3) . .
O19 W3 O17 K2 85.3(10) . .
O1 W3 O17 K2 28.5(3) . .
O14 W3 O17 K2 111.2(3) . .
O17 K2 O17 W2 -155(3) 3_757 .
O5 K2 O17 W2 -156.4(2) 3_757 .
O5 K2 O17 W2 23.6(2) . .
O1 K2 O17 W2 -74.6(3) 3_757 .
O1 K2 O17 W2 105.4(3) . .
O3 K2 O17 W2 -114.6(3) 3_757 .
O3 K2 O17 W2 65.4(3) . .
O17 K2 O17 W3 77(3) 3_757 .
O5 K2 O17 W3 75.3(3) 3_757 .
O5 K2 O17 W3 -104.7(3) . .
O1 K2 O17 W3 157.0(2) 3_757 .
O1 K2 O17 W3 -23.0(2) . .
O3 K2 O17 W3 117.0(3) 3_757 .
O3 K2 O17 W3 -63.0(3) . .
O20 W3 O18 Mn1 -172.3(4) . .
O19 W3 O18 Mn1 84.4(5) . .
O17 W3 O18 Mn1 -73.7(4) . .
O1 W3 O18 Mn1 3.9(10) . .
O14 W3 O18 Mn1 -1.4(3) . .
O20 W3 O18 K3 -12.5(5) . .
O19 W3 O18 K3 -115.9(5) . .
O17 W3 O18 K3 86.0(4) . .
O1 W3 O18 K3 163.6(6) . .
O14 W3 O18 K3 158.4(5) . .
O21 Mn1 O18 W3 -95.1(5) . .
O22 Mn1 O18 W3 11(2) . .
O15 Mn1 O18 W3 78.4(4) . .
O24 Mn1 O18 W3 171.1(4) . .
O14 Mn1 O18 W3 1.4(3) . .
W2 Mn1 O18 W3 47.7(3) . .
O21 Mn1 O18 K3 100.8(4) . .
O22 Mn1 O18 K3 -153.0(17) . .
O15 Mn1 O18 K3 -85.7(3) . .
O24 Mn1 O18 K3 7.0(3) . .
O14 Mn1 O18 K3 -162.7(3) . .
W2 Mn1 O18 K3 -116.4(2) . .
O26 K3 O18 W3 51.1(5) . .
O8 K3 O18 W3 130.1(4) 1_455 .
O10 K3 O18 W3 -144.8(4) 3_656 .
O20 K3 O18 W3 6.4(8) 3_657 .
O24 K3 O18 W3 -167.4(5) . .
O26 K3 O18 W3 -29.6(5) 3_657 .
O26 K3 O18 Mn1 -147.5(5) . .
O8 K3 O18 Mn1 -68.5(4) 1_455 .
O10 K3 O18 Mn1 16.6(4) 3_656 .
O20 K3 O18 Mn1 167.8(4) 3_657 .
O24 K3 O18 Mn1 -5.9(3) . .
O26 K3 O18 Mn1 131.9(4) 3_657 .
O20 W3 O19 W3 140.9(13) . 4_565
O18 W3 O19 W3 -115.3(13) . 4_565
O17 W3 O19 W3 -15(2) . 4_565
O1 W3 O19 W3 42.4(13) . 4_565
O14 W3 O19 W3 -39.3(13) . 4_565
O18 W3 O20 K3 21.1(9) . 3_657
O19 W3 O20 K3 117.4(8) . 3_657
O17 W3 O20 K3 -71.8(9) . 3_657
O1 W3 O20 K3 -157.4(8) . 3_657
O14 W3 O20 K3 -61(2) . 3_657
O22 Mn1 O21 Mn1 -58.3(8) . 4_565
O15 Mn1 O21 Mn1 30(4) . 4_565
O18 Mn1 O21 Mn1 112.6(8) . 4_565
O24 Mn1 O21 Mn1 -156.9(8) . 4_565
O14 Mn1 O21 Mn1 36.6(8) . 4_565
W2 Mn1 O21 Mn1 34.5(11) . 4_565
O22 Mn1 O21 K1 40.2(3) . .
O15 Mn1 O21 K1 129(3) . .
O18 Mn1 O21 K1 -148.8(3) . .
O24 Mn1 O21 K1 -58.3(3) . .
O14 Mn1 O21 K1 135.1(2) . .
W2 Mn1 O21 K1 133.1(3) . .
O16 K1 O21 Mn1 145.2(3) 3_656 4_565
O16 K1 O21 Mn1 -9.8(4) 2_656 4_565
O23 K1 O21 Mn1 67.7(3) . 4_565
O4 K1 O21 Mn1 67.7(3) 1_454 4_565
O25 K1 O21 Mn1 -79.7(4) 4_565 4_565
O25 K1 O21 Mn1 -144.9(4) . 4_565
O22 K1 O21 Mn1 31.8(3) 4_565 4_565
O22 K1 O21 Mn1 103.6(4) . 4_565
O16 K1 O21 Mn1 9.8(4) 3_656 .
O16 K1 O21 Mn1 -145.2(3) 2_656 .
O23 K1 O21 Mn1 -67.7(3) . .
O4 K1 O21 Mn1 -67.7(3) 1_454 .
O25 K1 O21 Mn1 144.9(4) 4_565 .
O25 K1 O21 Mn1 79.7(4) . .
O22 K1 O21 Mn1 -103.6(4) 4_565 .
O22 K1 O21 Mn1 -31.8(3) . .
O21 Mn1 O22 Mn2 54.8(6) . .
O15 Mn1 O22 Mn2 -118.6(5) . .
O18 Mn1 O22 Mn2 -51(2) . .
O24 Mn1 O22 Mn2 148.7(5) . .
O14 Mn1 O22 Mn2 -42.1(5) . .
W2 Mn1 O22 Mn2 -87.5(5) . .
O21 Mn1 O22 K1 -45.4(4) . .
O15 Mn1 O22 K1 141.2(3) . .
O18 Mn1 O22 K1 -151.7(17) . .
O24 Mn1 O22 K1 48.5(3) . .
O14 Mn1 O22 K1 -142.3(2) . .
W2 Mn1 O22 K1 172.26(18) . .
O13 Mn2 O22 Mn1 39(3) 4_565 .
O13 Mn2 O22 Mn1 118.9(5) . .
O22 Mn2 O22 Mn1 -53.8(6) 4_565 .
O23 Mn2 O22 Mn1 -144.9(5) . .
O11 Mn2 O22 Mn1 42.2(5) . .
W5 Mn2 O22 Mn1 42.0(7) 4_565 .
W5 Mn2 O22 Mn1 88.3(5) . .
O13 Mn2 O22 K1 144(2) 4_565 .
O13 Mn2 O22 K1 -135.8(3) . .
O22 Mn2 O22 K1 51.5(3) 4_565 .
O23 Mn2 O22 K1 -39.7(3) . .
O11 Mn2 O22 K1 147.4(2) . .
W5 Mn2 O22 K1 147.3(2) 4_565 .
W5 Mn2 O22 K1 -166.44(14) . .
O16 K1 O22 Mn1 -101.3(3) 3_656 .
O16 K1 O22 Mn1 115.1(3) 2_656 .
O23 K1 O22 Mn1 169.6(3) . .
O4 K1 O22 Mn1 -154.4(2) 1_454 .
O25 K1 O22 Mn1 27.8(5) 4_565 .
O25 K1 O22 Mn1 -36.7(4) . .
O22 K1 O22 Mn1 97.0(3) 4_565 .
O21 K1 O22 Mn1 32.1(2) . .
O16 K1 O22 Mn2 123.6(3) 3_656 .
O16 K1 O22 Mn2 -19.9(3) 2_656 .
O23 K1 O22 Mn2 34.5(2) . .
O4 K1 O22 Mn2 70.6(3) 1_454 .
O25 K1 O22 Mn2 -107.2(4) 4_565 .
O25 K1 O22 Mn2 -171.8(4) . .
O22 K1 O22 Mn2 -38.0(3) 4_565 .
O21 K1 O22 Mn2 -102.9(3) . .
O13 Mn2 O23 K1 -135.3(2) 4_565 .
O13 Mn2 O23 K1 135.3(2) . .
O22 Mn2 O23 K1 45.3(2) . .
O22 Mn2 O23 K1 -45.3(2) 4_565 .
O11 Mn2 O23 K1 180.000(4) . .
W5 Mn2 O23 K1 -140.07(16) 4_565 .
W5 Mn2 O23 K1 140.07(16) . .
O16 K1 O23 Mn2 -99.04(18) 3_656 .
O16 K1 O23 Mn2 99.04(18) 2_656 .
O4 K1 O23 Mn2 180.0 1_454 .
O25 K1 O23 Mn2 86.4(6) 4_565 .
O25 K1 O23 Mn2 -86.4(6) . .
O22 K1 O23 Mn2 31.45(17) 4_565 .
O22 K1 O23 Mn2 -31.45(17) . .
O21 K1 O23 Mn2 0.0 . .
O21 Mn1 O24 K3 -99.0(4) . .
O22 Mn1 O24 K3 170.1(3) . .
O15 Mn1 O24 K3 80.2(3) . .
O18 Mn1 O24 K3 -6.7(3) . .
O14 Mn1 O24 K3 29.5(10) . .
W2 Mn1 O24 K3 72.7(3) . .
O26 K3 O24 Mn1 47.9(4) . .
O8 K3 O24 Mn1 138.0(3) 1_455 .
O10 K3 O24 Mn1 -154.5(3) 3_656 .
O20 K3 O24 Mn1 -168.9(4) 3_657 .
O18 K3 O24 Mn1 5.2(2) . .
O26 K3 O24 Mn1 -61.5(5) 3_657 .
O8 K3 O26 K3 136.6(3) 1_455 3_657
O10 K3 O26 K3 121.9(10) 3_656 3_657
O20 K3 O26 K3 62.1(3) 3_657 3_657
O18 K3 O26 K3 -97.5(3) . 3_657
O24 K3 O26 K3 -136.1(3) . 3_657
O26 K3 O26 K3 0.0 3_657 3_657
